Upcoming SlideShare
×

# Welding lectures 7 8

907 views

Published on

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total views
907
On SlideShare
0
From Embeds
0
Number of Embeds
1
Actions
Shares
0
41
0
Likes
0
Embeds 0
No embeds

No notes for slide

### Welding lectures 7 8

1. 1. 9/20/2012Casting, Forming & WeldingCasting Forming & Welding (ME31007)  J u au Jinu Paul Dept. of Mechanical Engineering 1 1 Welding Lecture ‐ 7 g 13 Sept 2012, Thursday 8.30 ‐9.30 am Arc Welding- Electrical features 2 2 1
2. 2. 9/20/2012Arc Electrical Features-impedance• An electric welding arc is an impedance (related to the resistance of a circuit, but including contributions f t ib ti from capacitance and i d t it d inductance as well) to the flow of electric current• Specific impedance at any point in an arc is inversely proportional to the density of the charge carriers and their inherent mobility.• The total impedance depends on the radial and p p axial distribution of charge carrier density• The impedance of the plasma column is a function of temperature (except regions near the arc terminals) 3 3 Arc-Electrical features Electrode Plasma Work • All electric arcs consist of three regions – the cathode fall space (or drop zone); – the plasma column fall space (or drop zone) – the anode fall space (or drop zone) 4 4 2
3. 3. 9/20/2012 Arc-Electrical features • Electrical power dissipated in each regions of the arc given by P = I(Ea + Ec + Ep) where Ea is anode voltage, Ec is cathode voltage, and Ep is plasma column voltage • Intermediate regions  Involved in expanding or contracting the cross section of the gaseous conductor to accommodate each of these main regions. i • As a consequence, welding arcs assume bell or cone shapes and elliptical or some other noncylindrical contour. 5 5 Arc Shape ElectrodeArc shape = Interaction of(plasma + Arc + Ambience) Plasma • Bell Shape • Cone • Elliptical Work • Cylindrical 6 6 3
4. 4. 9/20/2012 Arc Shape- Influencing factors1. Shape of the arc terminals (i.e., pointed welding electrode producing a narrow arc f d i focused at d t the electrode tip and flat work piece electrode, which causes the arc to spread)2. Gravitational forces3. Magnetic forces (from both g ( internally generated and externally induced or applied sources)4. Interactions between the plasma and ambience (shielding gas) 7 7 7 Arc Shape- Influencing factors • N t Nature of electrode- C f l t d Consumable/non bl / consumable • Electrode coating/gas generation • Shielding gas • M Magnitude & polarity of current source it d l it f t 8 4
5. 5. 9/20/2012 Arc Shape (c) CO2 shielded  (a) GTA GMA welding  (b) SMA Non Consumable consumable Consumable electrode + l t d electrode + electrode + Gas Inert gas CO2 gas generation 9 9 Arc radiation• Arc radiation  amount and character depends on – the atomic mass and chemical composition of the gaseous medium, – the temperature, and the pressure.• Spectral analysis shows line and continuum emissions due to excited and ionized states of atoms and ions• Radiation  UV, visible, IR• Energy loss due to radiation  10-20 %• Highly hazardous to eyes, skin 10 10 5
6. 6. 9/20/2012 Metal transfer in Arc welding• The manner in which molten filler metal is transferred to the weld pool  profound effects on the performance of a consumable electrode arc welding process• These effects include – Ease of welding in various positions – Extent of weld penetration; p – Rate of filler deposition and – Heat input – Stability of the weld pool – Amount of spatter loss 11 Mode of Metal transfer-Influencing parameters• Pressure generated by the evolution of gas at the electrode ti (for fl t th l t d tip (f flux-coated or fl t d flux- cored electrode processes)• Electrostatic attraction between the consumable electrode and the workpiece• Gravity y• “Pinch effect” caused near the tip of the consumable electrode by electromagnetic field forces  spray 12 6
7. 7. 9/20/2012 Mode of Metal transfer-Influencing parameters• Explosive evaporation of a necked region formed between the molten drop and solid portions of the electrode due to very high conducting current density• Electromagnetic action produced by divergence of current in the arc plasma around a drop.• Friction effects of the plasma jet (plasma friction)• Surface tension effects once the molten drop (or electrode tip) contacts the molten weld pool 13 Metal transfer types• Free-flight transfer: Complete detachment of the molten metal drop from the consumable electrode  flight to the work piece and weld pool, without any direct physical contact• Bridging transfer: molten metal drops are never completely free; rather they are always attached to the th consumable electrode and th bl l t d d the workpiece, momentarily bridging the two from a material standpoint - and electrically• Slag-protected transfer 14 7
8. 8. 9/20/2012 Free-flight-Globular Transfer• Low welding currents (50-170 A) in p pure argon, molten metal from a g small diameter solid steel wire electrode is transferred in the form of globules• Drops diameter larger than the wire• Large drops  detach by gravity• Low rate of globule formation, detachment, and transfer (< 1-10 s-1)• Globular transfer  down-hand position 15 Free flight: Globular-projected Transfer• As the welding current increases within the range of 50-170A the 50 170A, drops become progressively smaller,  electromagnetic forces are having an increasing effect on detachment• For DCEP, drop size 1/ welding current. current• As welding current is increased, the rate of drop transfer also increases 16 8
9. 9. 9/20/2012 Free-flight transfer modes Increasing current Individual drop formation and detachment sequence in (a) globular transfer and (b) projected and (c) streaming axial spray transfer 17 Free flight -Spray Transfer/streaming transfer• At current > critical level  No individual drops• Tip of the consumable electrode becomes pointed  cylindrical stream of liquid metal flows toward the work piece in line with the electrode.• Near its tip (nearest the work piece), piece) this cylinder disperses into many very small droplets  Electromagnetic pinch effect• The rate at which droplets are transferred is hundreds per second. 18 9
10. 10. 9/20/2012 Free flight -Spray Transfer: Features • Axial spray transfer mode  Excellent stability, virtually free of spatter • Droplets are actively propelled away from the consumable electrode and into the molten weld pool to be captured by surface tension force. • Droplets are transferred in line with the electrode  Filler metal can be directed exactly where it is needed. needed • This is a great advantage when making vertical or overhead welds, where the propelling force offsets the disruptive effect of gravity 19 Bridging or short circuiting transfer• Large dia. Electrodes  too high transition current to achieve axial spray transfer (e.g., 200-220A for 1-mm- diameter steel wire)  Bridging transfer• Voltage is kept low (say 17-21 V versus 24-28 V for globular transfer with steel wires)• The tip of the electrode periodically dipped into the molten weld pool. 20 10
11. 11. 9/20/2012 Bridging or short-circuiting transfer• Bridging  Molten metal transfer by a combination of surface tension and electromagnetic forces• Low voltage reduces the rate at which the electrode is melted• In the presence of carbon dioxide (CO2) in shielding gas, the molten drop at the electrode tip is p p p pushed upward  repelled transfer. In this case, short-circuiting captures the drop before it detaches in an unfavorable manner 21 Short-circuiting transfer- Advantages • Less fluid molten metal (due to ( less superheat) • Less penetration (due to lower welding voltage and lower net energy input). • Easy handling in all positions, especially overhead and for the overhead, joining of thin-gauge materials. • Minimum Spatter 22 11
12. 12. 9/20/2012 Sequence of short-circuiting transfer(a) globule of molten metal builds up on the end of the electrode; (b)globule contacts surface of weld pool; (c) molten column pinches off todetach globule; and (d) immediately after pinch-off, fine spatter may result 23 Short-circuiting transfer: I-V trace 24 12
13. 13. 9/20/2012 Pulsed arc or pulsed current transfer• Steady current to maintain the arc and a periodic current pulse to a higher level• Periodic pulses detaches a drop and propels it into the weld pool,• Advantage of axial spray transfer at a lower average current, and, thus, lower net heat input.• The time period of pulses must be short enough to suppress globular transfer, but long enough to ensure that transfer by the spray mode will occur 25 PULSED-CURRENT TRANSFER 26 13
14. 14. 9/20/2012 Pulsed current transfer• This pulsed mode differs from the normal spray mode in that – Th molten metal transfer is interrupted between the The lt t lt f i i t t db t th current pulses – The current to produce spray is below the normal transition current• Pulse shape (i-e., wave form, especially the rate of the rise and fall of current) and frequency can be varied over a wide range in modern, solid- g state power sources• Rate of molten metal transfer can be adjusted to be one drop or a few drops per pulse (by adjusting the pulse duration) 27 Classification of transfer modes 28 14
15. 15. 9/20/2012 Dominant forces in transfer modes 29Effect of welding process parameters on transfer modes-Summary • Current at which transition from globular to spray transfer begins depends on – Composition of the consumable electrode, – Electrode diameter, – Electrode extension, – Composition of shielding gas. • Shielding Gas Effects • Process Effects • Operating Mode or Polarity Effects 30 15
16. 16. 9/20/2012 Welding ecture Welding Lecture ‐ 8 20 Sept 2012, Thursday 8.30 am ‐9.30 am Welding Processes‐ Resistance welding Resistance welding 31 31 Resistance welding (RW)• Generate heat through the resistance to the flow of electric current in parts being welded ti t b i ld d• The parts are usually an integral part of the electrical circuit• Contact resistance  heats the area locally by I2R,  melting  formation of a nugget• C t t resistance must be Contact i t tb higher at the point to be welded than anywhere else. 32 32 16
17. 17. 9/20/2012Resistance welding 33 33Resistance welding 34 17
18. 18. 9/20/2012 Resistance welding• Pairs of water-cooled copper electrodes• Apply pressure – To reduce the contact resistance at the electrode-to-workpiece interface i t f – Contain the molten metal in the nugget – To literally forge the work surfaces together in the vicinity of the weld• The principal process variables – welding current (several thousands to tens of thousands of amperes) – welding time (of the order of s) – electrode force and electrode shape• DC power (provided from either single-phase or ( id d f ith i l h three-phase AC line 440-480 V using step-down transformer/rectifiers)• Usually used to join overlapping sheets or plates as lap joints, which may have different thicknesses 35 35 Resistance welding-types • Resistance spot welding ( S ) es sta ce e d g (RSW) • Resistance seam welding (RSEW) • Projection welding (PW) • Flash welding (FW) • Upset welding (UW) • Percussion welding (PEW) 36 36 18
19. 19. 9/20/2012 Resistance spot welding (RSW)• Series of discrete nuggets produced by resistance heating• Nuggets (welds) are usually produced directly under the electrodes,  Not necessarily if there is another more favourable path (shunt), for the current 37 37 Series resistance spot welding 38 38 19
20. 20. 9/20/2012 Resistance welding cycle• Squeeze Time: Time interval between timer initiation and the first application of current needed to assure that electrodes contact the work and establish full force• Weld time: The time for which welding current is applied (in single impulse welding) to the work• Hold Time: The time during which force is maintained on the work after the last impulse of welding current ends to allow the weld nugget to solidify and develop strength.• Off Time: The time during which the electrodes are off the work and the work is moved to the next weld location for repetitive welding. 39 Pressure-current cycle 40 40 20
21. 21. 9/20/2012 Pressure-current cycle 1. Off time: Parts inserted between open electrodes, 2. 2 Squeeze Ti S Time:Electrodes close and f El t d l d force iis applied, 3. Weld time— current is switched on, 4. Hold time: Current is turned off but force is maintained or increased (a reduced current is sometimes applied near the end of this step for stress relief in the weld region), and 5. Off time: Electrodes are opened, and the welded assembly is removed. 41 41 Enhanced welding cycle1. Pre-compression force is used to set electrodes and work pieces together2. Preheat is2 P h t i applied t reduce th li d to d thermal gradients at l di t t the start of weld time or to soften coatings3. Forging force is used to consolidate weld nugget4. Quench and temper times are used to produce desired weld properties in hardenable steels;5. Post heat is used to refine weld nugget grain size and improve strength6. Current decay is used to retard cooling of aluminum alloys to help prevent cracking 42 21
22. 22. 9/20/2012Enhancedresistanceweldingcycle 43 Nugget formation Nugget formation and heat dissipation into the surrounding base metal and electrodes during resistance spot welding 44 22
23. 23. 9/20/2012 Optimum current, time in RW• Optimum current and weld time for maximum shearstrength of the RW joint 45 Resistance seam welding Conventional resistance seam Roll spot Continuous C tiwelding, in which welding resistanceoverlapping spots seam are produced 46 46 23
24. 24. 9/20/2012Resistance seam welding 47 Mash seam weld 48 48 24
25. 25. 9/20/2012 Projection welding (PW),• Projections or dimples in overlapping joint elements  concentrate the current during welding, focusing the weld energy and helping to locate the weld more precisely• Contact points determined by the design of the parts to be joined  may consist of projections, embossments, or localized intersections of the parts 49 49 Flash welding(FW)1. Normally used for butt joints  the two surfaces y j to be joined are brought into near contact 2. Electric current is applied to heat the surfaces to the melting point  the surfaces are forced together to form the weld 50 50 25
26. 26. 9/20/2012 Upset welding (UW)• Upset welding (UW) is similar to flash welding• H ti i UW i Heating in is accomplished entirely by electrical resistance at the contacting surfaces; no arcing occurs.• Not a fusion-welding process• Applications of UW & FW- joining ends of wire, pipes, tubes etc. 51 51 Percussion welding• Resistance heating by the rapid release of electrical energy from a storage device ( g , capacitor). g (e.g., p )• Similar to flash welding, except that the duration of the weld cycle is extremely short, ~ 1 to 10 ms• Very localized heating  attractive for electronic applications in which the dimensions are very small 52 52 26